Do you need custom fasteners created with 13-8 MO? Since our inception, Vegas Fastener Group has met every challenge of providing Quality, Timely, Cost-effective solutions for specialty fastener applications. Every product is built to your specifications, using your prints if necessary.
Below are the technical specifications of the 13-8 MO Bar Stock we have available to meet your needs.
Special Metals Nickel 200
Subcategory: Metal; Nickel Alloy; Nonferrous Metal; Pure Metallic Element Key Words: ASME SB-160 – SB-163, Boiler Code Sections III, VIII, IX; DIN 17740, 17750-17754, Nickel, Ni, UNS N02200; BS 3072-3076 (NA11); ASTM B 160 – B 163, B 725, B 730, Werkstoff Nr. 2.4060, 2.4066
Material Notes: Nickel content above includes cobalt. Commercially pure (99.6%) wrought nickel with good mechanical properties and resistance to a range of corrosive media. Good thermal, electrical, and magnetostrictive properties. Ferromagnetic. Used for a variety of processing equipment, particularly to maintain product purity in handling foods, synthetic fibers, and alkalis. Standard product forms are round, flats, pipe, tube, plate, sheet, forging stock, strip, and wire.
Data provided by the manufacturer, Special Metals.
MicroGroup’s inventory of small diameter 304 and 316 and other stainless steel, nickel based alloys, and titanium alloys exceeds 5 million feet. Redraw of material to specific sizes and shapes, as well as secondary operations to convert tubing into components and assemblies. Visit http://www.microgroup.com or Phone 1-800-ALL-TUBE (1-800 255-8823) or 1-508-533-4925.
|Density||8.89 g/cc||0.321 lb/in³|
|Tensile Strength, Ultimate||462 MPa||67000 psi||Annealed. Value at room temperature. Value at 300°C is 475 MPa.|
|Tensile Strength, Yield||148 MPa||21500 psi||Annealed. Value at room temperature; 0.2% offset. Value at 300°C is 120 MPa.|
|Elongation at Break||45 %||45 %||Annealed. Value at room temperature. Value at 300°C is 48%.|
|Electrical Resistivity||9.6e-006 ohm-cm||9.6e-006 ohm-cm|
|Curie Temperature||360 °C||680 °F|
|CTE, linear 20°C||13.3 µm/m-°C||7.39 µin/in-°F||20-100°C|
|Heat Capacity||0.456 J/g-°C||0.109 BTU/lb-°F|
|Thermal Conductivity||70.2 W/m-K||487 BTU-in/hr-ft²-°F|
|Melting Point||1435 – 1446 °C||2620 – 2630 °F|
|Solidus||1435 °C||2620 °F|
|Liquidus||1446 °C||2630 °F|
This information is provided by MatWeb.com, The Online Materials Database and is reprinted with their permission.
Copyright 1996-2014 by Automation Creations, Inc. The contents, results, and technical data on this page may not be reproduced either electronically, photographically or substantively without permission from Automation Creations, Inc and MatWeb.com. No warranty, neither expressed nor implied, is given regarding the accuracy of this information. The user assumes all risk and liability in connection with the use of information from MatWeb.com.